Copper pad dissolution and microstructure analysis of reworked plastic grid
Copper Pad Dissolution and Microstructure Analysis of Reworked Plastic Grid
Lei Nie, Michael Osterman and Michael Pecht
Center for Advanced Life Cycle Engineering (CALCE)
University of Maryland
College Park, MD
Phone: 301-405-5323, Fax: 301-314-9269
An experimental study was conducted to examine the impact of rework processes on quality and reliability. In this study,
676 IO plastic ball grid array packages were assembled with Sn3.0Ag0.5Cu solder paste and eutectic SnPb solder paste.
Selected parts on circuit boards were subjected to rework processes one time, three times and five times. X-ray inspection
and environmental scanning electron microscope were used to investigate impact of part replacement on the ball grid array
voids, the microstructure of intermetallic compound, and copper pads. Since the rework process includes multiple liquid
solder state periods, it consumes more copper and makes the intermetallic compound growth trend an interesting topic.
Copper pad dissolution was found in the samples after multiple rework processes. Lead-free assemblies consumed more
copper than mixed assemblies because of higher concentration of Sn in lead-free solder. The thickness of intermetallic layer
increased as the total rework time increased. Ultra thick intermetallic compound was found at the connection area between
the copper pad and the copper trace after the rework processes were applied three times and five times, which may lead to
The Directive on the Restriction of the Use of Certain Hazardous Substances in Electrical and Electronic Equipment (RoHS),
which became effective on July 1, 2006, mandates that electronics industries no longer use tin-lead solder. China, Japan, and
other countries have also published environmental regulations to restrict tin-lead solder -. At the same time, there are
exemptions for some products whose applications require high reliability. These exemptions have not impacted the
conversion of piece part suppliers to being lead-free.
Rework is defined as the correction of a defect before the printed board assembly leaves the plant, and repair is defined as the
correction of a defect found in the field . Since the electronic industry is now using the lead-free solder predominately, it
is important to understand the impact of rework process and reworked assemblies on reliability. Some literature addresses
copper dissolution in plated through-hole (PTH) barrels in the rework process -. This creates a concern because it is
possible for a hidden defect to be present after reworking PTH assemblies. Currently, no literature has focused on the copper
dissolution of reworked ball grid array (BGA) assemblies, which is another possible hidden defect.
Assemblies formed by the mixing of SnPb and Pb-free material are termed “mixed assemblies”. Many studies have focused
on the microstructures of mixed and lead-free solder interfaces -. The microstructure of mixed assemblies formed by
lead-free BGAs and tin lead solder paste is related to the volume of solder paste. The intermetallic compound (IMC) growth
during the isothermal aging condition is well understood. A driving force of this phenomena is solid solder/solid pad
interdiffusion. The rework process includes multiple liquid solder state periods, which makes the IMC growth trend an
In this study, 676 IO BGAs with Sn3.0Ag0.5Cu (SAC305) solder balls were assembled with SAC305 and eutectic solder
paste. Individual locations on the printed circuit boards (PCBs) were subjected to rework one time, three times and five times.
X-ray inspection was used to investigate BGA solder voids. Parts were cross-sectioned to inspect the consumption of copper
pads and the morphology of IMC. An environmental scanning electron microscope (ESEM) and an energy-dispersive x-ray
spectroscopy (EDS) were used to investigate the growth of IMC, as well as the composition of IMC.A set of test boards was
designed and manufactured to test the effect of multiple rework processes on the reworked assemblies. The components
assembled on the board were 676 IO BGAs with SAC solder balls. There were two kinds of assemblies, those using pure
lead-free solder (SAC BGA and SAC solder paste) and those using mix-solder (SAC BGA and tin-lead solder paste).
Six BGAs were assembled on each board as shown in Figure 1. Three locations were selected to be reworked (see Figure 1).
These three locations were first reworked one time. Then two of the three locations were reworked another two more times,
and the last location was reworked two more times. Thus, there were three treatments for these BGA assemblies locations:
one replacement, which means remove the BGAs on the PCB and replace a new BGA; three replacements, which means
remove the BGAs three times, and every time replace a new BGA on the PCB; and five replacements, which means remove
the BGAs five times, and every time replace a new BGA on the PCB. Table 1 lists the test matrix of reworked assemblies.
The PCB assemblies were subjected to preconditioning at 100°C for 24 hours before being reworked and between each
Figure 1: 676 IO BGA assemblies
Table 1: Rework test matrix of 676 IO BGAs
SnPb SnPb 3
SAC SAC 3
The rework process of surface mount technology (SMT) components involves four steps: component removal, site redressing,
component placement, and component reflow. To remove the components assembled on the PCB, a thermal profile needs to
be set up to melt the solder. A thermal profile is established by various trial runs, as it depends on several factors such as
board thickness, type of solder and component size.
A VJ Electronix SRT1800 rework station with a bottom heater and a hot nitrogen nozzle on top was used to replace the BGA
components. The hot nitrogen nozzle was applied to each assembled BGA to heat up the solder, and at the peak temperature,
when the solder melted, the component was removed by suction using a vacuum tool.
After the components were removed from the PCB, residue solder may be left on the pads. The pads must have a flat surface
to insure the quality of replacement. In this study, the soldering iron and wick method was used to remove the residue solder
from the pads. A fluxed copper braid was heated by the soldering iron and brushed over the pads. The heated braid melted
the residue solder, and the solder was wicked up into the copper braid. Figure 2 shows the pads after site redressing. The
pads showed a clean surfaces and solder mask were not damaged during the removal procedure.
Once the site was redressed, a mini-stencil was aligned and placed on the location, and the solder paste was printed on the
pads. This mini-stencil was similar in size to the component and had openings that matched the pads. The lead-free rework
used of Alpha OM-338 (SAC305), a type of lead-free, no-clean solder paste. The mixed solder rework used Indium SMQ-
92J (6337), a no-clean, tin-lead solder paste. After solder paste was applied to pads, components were aligned and placed by
semi-automated techniques to the locations. The hot nitrogen nozzle was placed above the components to melt the solder
balls and solder paste. The new BGAs were assembled on the PCBs after cooling.
Figure 2: Pads inspection after site redressing
(a) PCB pads of mixed assemblies; (b) PCB pads of lead-free assemblies
3 Results and Discussion
The non-reworked and reworked components were examined by X-ray inspection to assess the assembled and reworked
quality. Then assembled BGAs were cut, molded, and cross-sectioned to investigate the copper pads and the intermetallic
layer using environmental scanning electron microscope (Quanta FEG ESEM 200).
3.1 Void Calculation in Reworked and Non-Reworked Assemblies
IPC-7095  offers information on BGA voids, including their sources, impact, detection, and elimination. Large voids can
lead to reliability problems since a reduced cross-section of solder area has lower heat transfer, mechanical load burdening,
and current carrying capability. X-ray inspection is the common detection equipment used to measure the void’s percentage.
Total voids larger than 30% of the solder ball diameter are considered unacceptable. The void’s percentage can be the size of
one void or the sum of the sizes of many voids.
Figure 3: The calculation of void’s percentage of non-reworked and reworked BGAs
X-ray inspection was used to detect the voids in non-reworked and reworked BGAs. For each BGA, 80 solder balls were
examined from the four corners and the central part of the BGA to calculate the percentage of the voids. Figure 3 lists all of
the voids’ percentages in non-reworked and reworked BGAs. (The lines inside the rectangular box represent roughly the
middle 50% of the data, and whiskers extend to either side indicating the general extent of the data. The stars refer to the
outliers.) The lead-free assembled non-reworked BGA had a lower void percentage compared to the mixed assembled non-
reworked BGA. But, after five replacements, the mixed assembled BGA had a lower void percentage than that of a pure
lead-free assembled BGA. None of the BGAs failed the void’s percentage calculation.
3.2 Copper Pad Dissolution
When a new component was attached to the pads during the rework process, reactions occurred between the solder balls and
the PCB pads. Cu dissolved into liquid Sn and formed an intermetallic layer at the solder/pad interface. Hamilton and
Snugovsky  addressed the Cu dissolution during the lead-free PTH rework process. They found that the copper pad
dissolution rate of the lead-free (SAC) rework process was higher than that of the eutectic tin-lead rework process.
In this study, the copper pad thicknesses of lead-free and mixed assembly joints were measured using ESEM. For each
sample, 27 measurements were documented. The results are plotted in Figure 4. The copper pad thicknesses of the non-
reworked lead-free (SAC) assemblies and the non-reworked mixed assemblies were initially equal. However, after five
replacements, the copper pad thickness of the lead-free (SAC) assemblies was only about 50% that of the mixed assemblies
(see Figure 5 and Figure 6).
0 1 3 5
Number of Rework
Figure 4: Copper thickness of lead-free and mixed assemblies
During the reflow process, liquid Sn and solid Cu reacted with each other to form intermetallic compounds at the solder/pad
interface. Cu dissolves into liquid Sn very fast (in seconds), and there is a large driving force for the chemical reaction
between Cu and Sn. The Cu-Sn IMC formation mechanism is controlled by the dissolution of Cu into liquid Sn followed by
chemical reactions .
In SnAgCu solder, the concentration of Sn is higher than in SnPb solder. Higher concentration of Sn leads to higher Cu
dissolution. Thus, the SnAgCu solder can dissolve more Cu than SnPb solder. In eutectic SnPb solder, Pb can be considered
a solvent, which decreases the concentration of Sn. In mixed assemblies, when the Cu dissolves into bulk solder, the local Pb
concentration will increase at the IMC/bulk solder interface, which blocks Cu dissolved into bulk solder. Thus, the loss of
copper pad in lead-free assemblies is more than that in mixed assemblies.
Figure 5: Solder/pad interface in lead-free
assemblies after five replacements
Figure 6: Solder/pad interface in mixed
assemblies after five replacements
3.3 Over-Consumption of Copper Pad
The design of copper pads allows them to be electrically interconnected with different solder balls (see Figure 7). Figure 8
shows the schematic images of copper pad connections; the red circle indicates the site of over-consumption. During the
rework process, the heat tends to conduct along the copper, since copper has very good thermal conductivity. Not much heat
was conducted from the copper pad to the copper trace since the connection site between them was narrower compared to the
area of copper pads. Thus, heat concentrated in the connection site led to thicker intermetallic compound formation and over-
consumption of copper pad after multiple replacements. There is no copper pad over-consumption in the samples after one
and three replacements, but the heat accumulation led to copper over-consumption after five replacements.
Figure 7: Backscattered electron images of two
solder balls connection by the copper pads
(mixed assemblies, 1 replacement)
Figure 8: Schematic images of heat transfer
between the Cu pads and the Cu trace on a PCB
The consumption of the copper pad was relatively even for the parts after one and three replacements. However, the edge of
the copper pad in the parts with five replacements was over-consumed. Figure 9 shows the backscattered electron images of
the edge of the copper pads for the reworked lead-free and mixed assemblies. Both the lead-free and the mixed assemblies
had similar copper over-consumption trends. After one replacement, the copper pads of the samples were relatively even;
after three replacements, they had a small amount of over-consumption at the edge; after five replacements, they were almost
consumed, and the intermetallic compound replaced the copper.
Copper Pad on PCB
Copper Pad on PCB
Cu Pad Cu PadCu Trace
Copper pad on PCB
Pad of component
Solder ball Solder ball
Pad of component
Heat Transfer Direction
(a) (b) (c)
(d) (e) (f)
Figure 9: Backscattered electron images of the edge of the copper pad
(a) lead-free assemblies, one replacement; (b) lead-free assemblies, three replacements;
(c) lead-free assemblies, five replacements; (d) mixed assemblies, one replacement;
(e) mixed assemblies, three replacements; (f) mixed assemblies, five replacements.
3.4 Interfacial Intermetallic Compound Morphology
At the temperature of the reflow process, Cu6Sn5 is the first phase to form at the liquid Sn/Cu interface. The formation of
Cu6Sn5 takes place within seconds. Cu dissolves into liquid Sn, and reacts with liquid Sn. An ultra-thin layer of Cu3Sn
forms between the Cu6Sn5 and the Cu pad, but it is too thin to be detected . However, the Cu3Sn becomes thicker after
long periods of isothermal aging . The melting temperatures of Cu6Sn5 and Cu3Sn are 415 °C and 638 °C respectively
. Thus, the interfacial intermetallic compounds (IMC) can remain in the residue solder, since the highest temperature is
lower than 300°C during the solder removal process. When a new component attaches to the pad and reflows, a new IMC
layer forms at the solder/pad interface. The interfacial IMC morphology of reworked parts is thus different from the as-
assembled parts (see Figure 10).
The interfacial IMC of as-assembled joints was scallop shaped Cu6Sn5, and Cu3Sn was not detected, perhaps due to the
resolution of the ESEM. Unlike the continuous layer of IMC undergoing isothermal aging, a much thicker layer of IMC with
a fragmentary shape was found at the interface of the sample after five replacements. The morphology of the IMC is related
to the thermal process the parts experienced. The reworked parts went through reflow processes and isothermal aging (100°C,
24 hours) several times. The kinetic force of IMC growth during reflow was liquid Sn/solid Cu interdiffusion, while the
kinetic force during isothermal aging was solid Sn/solid Cu interdiffusion. The difference in driving forces led to multiple
layers of IMC formation at the interface of the solder/pad in the reworked samples. In the ESEM images, the morphology of
the IMC appears fragmentary.
Figure 10: Backscattered electron images of IMCs at solder/pad interface
(a) Lead-free assemblies, as-assembled; (b) Lead-free assemblies, five replacements;
(c) Mixed assemblies, as-assembled; (d) Mixed assemblies, five replacements.
3.5 Interfacial Intermetallic Compound Thickness
Figure 10 shows that the interfacial IMC layer became thicker after the rework process for both lead-free and mixed
assemblies. Figure 11 plots the interfacial IMC thickness of lead-free and mixed assembly joints for as-assembled and
reworked samples. The interfacial IMCs growth of lead-free assemblies after rework process was much faster than the
growth of the interfacial IMCs undergoing thermal aging conditions (normally below 150°C) . A similar trend was found
among mixed assembly samples; the interfacial IMC layer was much thicker than the interfacial IMC undergoing isothermal
aging conditions. This was due to different thermal processes: isothermal aging and rework.
The driving force of interfacial IMC growth undergoing the isothermal aging condition is solid/solid interdiffusion, which is
much slower than solid/liquid interdiffusion. In one rework process, there were three periods when the solder became liquid:
component removal, site redressing, and component reflow. Prolonged liquid time enhances the interfacial IMC growth,
which leads to much thicker interfacial IMC in comparison to the interfacial IMC undergoing thermal aging.
Cu pad on PCB
Cu pad on PCB
Cu pad on PCB
Cu pad on PCB
0 1 3 5
Number of Rework
Figure 11: IMC thickness of lead-free and mixed assemblies after multiple rework processes
In this study, 676 IO PBGAs with Sn3.0Ag0.5Cu were assembled with Sn3.0Ag0.5Cu and eutectic Sn37Pb solder paste.
Three selected parts of each assembly were subjected to rework one time, three times, and five times. X-ray inspection and
ESEM were used to investigate the BGA voids, the IMC morphology, the IMC thickness, and the copper pad dissolution.
X-ray inspection results showed that none of the BGAs exceeded the criterion in the BGA voids calculation, according to the
IPC-7095. Copper pad dissolution was observed for joints of both lead-free and mixed assemblies after multiple rework
processes. The copper pad dissolution in joints of lead-free assemblies was found to be larger than that of mixed assemblies.
This is due to the higher concentration of Sn in the lead-free solder, which means there is a faster reaction between liquid
lead-free solder and Cu. Cu over-consumption was observed at the edge of pads after five replacements for both lead-free
and mixed assemblies. During the reflow process, heat concentrated at the connection site between the copper pads and the
copper traces, which led to the formation of ultra thick IMC and over-consumption of copper pad. Thick IMC and thin
copper pad may lead to reliability concerns. Thus, more than three rework processes is not recommended.
IMC morphology of reworked samples was different from that of aged samples. The IMCs presented a fragmentary
morphology due to multiple liquid solder periods, including component removal, site redressing, and component reflow. The
growth of IMCs was much faster than the growth of IMCs undergoing the isothermal aging condition due to the prolonged
liquid time in the rework process. Thus, reworked BGAs may have reliability concerns due to thicker IMC layer in real
The authors would also like to thank the members of the CALCE Electronic Product and Systems Consortium for sponsoring
work presented in this paper.
 S. Ganesan and M. Pecht, Lead-free Electronics, New York: John Wiley and Sons Inc., 2006.
 M. Pecht, Y. Fukuda, and S. Rajagopal, “The Impact of Lead-free Legislation Exemptions on the Electronics Industry,”
IEEE Transactions on Electronics Packaging Manufacturing, Vol. 27, No. 4, October 2004, pp. 221-232.
 L. Nie, M. Pecht, and R. Ciocci, “Regulations and Market Trends in Lead-free and Halogen-free Electronics,” Circuit
World, Vol. 33, No. 2, 2007, pp. 4-9.
 IPC 7711, “Rework of Electronic Assemblies”, North brook, IL, May 2002.
 K. Doss, A. Donaldson, A. Tong and R. Aspandiar, “Studies on The Removal of Copper during Minipot Rework with
different Lead-Free alloys”, Proceedings of SMTA International, October 11, 2007.
 A. Donaldson, “The Effect of Critical to Function Parameters of the Lead-Free Mini-Pot Through-Hole Connector
Rework Process on the Final Barrel Copper Thickness”, Proceedings of SMTA International, October 11, 2007.
 C. Hamilton and P. Snugovsky, “Have High Cu Dissolution Rates of SAC305/405 Alloys Forced A Change in The lead
Free Alloy Used During PTH Processes?”, Proceedings of the Pan Pacific Conference, January, 2007.
 C. Hamilton, P. Snugovsky and M. Kelly, “A Study of Copper Dissolution During Lead Free PTH Rework Using A
Thermally Massive Test Vehicle”, Circuits Assembly, May 1, 2007.
 P. Snugovsky, A.R. Zbrzenzny, M. Kelly and M. Romansky, “Theory and Practice of Lead-free BGA Assembly Using
Sn-Pb Solder”, Proceedings of CMAP International Conference on Lead-free Soldering, Toronto, Canada, May24-26,
F. Hua, R. Aspandiar, T. Rothman, C. Anderson, G. Clemons and M. Klier, “Solder Joint Reliability Of SnAgCu BGA
Components Attached with Eutectic SnPb Solder Paste”, Journal of Surface Mount Technology Association, Vol. 16,
Issue 1, 2003
A. Choubey, M. Osterman, and M. Pecht, “Microstructure and Intermetallics Formation in SnAgCu BGA Components
attached with SnPb Solder under Isothermal Aging”, IEEE Transactions on Device and Materials Reliability, Vol. 8,
Issue 1, 2008, pp 160-167.
IPC-7095, “Design and Assembly Process Implementation for BGAs”, August 2000.
T. Laurila, V. Vuorinen, and J.K. Kivilahti, “Interfacial Reactions between Lead-Free Solders and Common Base
Materials”, Materials Science and Engineering, R 49 (2005), pp. 1-60.
J.H. Shim, C.S. Oh, B.J. Lee and D.N. Lee, “Thermodynamic Assessment of the Cu-Sn System”, Z. Metallkd., Vol. 87,
No. 3, 1996, pp. 205-212.